The need to store electricity is becoming increasingly critical to link energy supply to our energy demands as we shift from the use of fossil fuels to renewable energy sources such as solar and wind. Advances in the past two decades in electro-chemical energy storage technologies such as Li-ion batteries have enabled the ubiquity of mobile electronic devices in our lives. The expansion of electriﬁ ed transportation to driving
ranges of ∼ 300 miles per recharge, as offered by vehicles
based on internal combustion engines, and the use of intermit-tent solar and wind energy for stationary power applications call for storage technologies with much greater gravimetric energies than Li-ion batteries. Energy storage schemes that involve the transfer of multiple electrons during discharge
such as lithium-air 1 and zinc-air batteries, 2 as well as Li-S
batteries (see the Nazar et al. article in this issue), can provide higher gravimetric energies than Li-ion batteries
that are constrained largely to one-electron intercalation. 1 – 3
Although the basic principle behind the operation of
metal-air batteries (or more accurately metal-O 2 since only the O 2
drawn from the air is used; other reactive constituents [e.g.,
CO 2 ] need to be excluded to a sufﬁ cient level) is well known,
there are immense challenges to overcome in order to make these technologies practical and to do so with a battery that delivers the promised step-change in energy storage. In this article, we discuss some key materials challenges and
high-light recent advances in Li-O 2 battery research.
The operation of Li-O 2 batteries is based on the
conver-sion of stored chemical energy in lithium (fuel) and oxygen into electrical energy via the formation of reaction products
containing lithium ions and reduced oxygen species. 4 – 6 This
scheme incorporates operational elements of a fuel cell
(e.g., reduction of gaseous O 2 from the environment during
discharge) with that of a battery (storage of electrons and Li +
in the oxygen electrode), and therefore represents a departure from conventional constraints of Li-ion positive electrode
development. Li-O 2 batteries differ from Li-ion batteries in
that rather than intercalating lithium into a host lattice con-taining transition metal ions (see the Introductory article in
this issue), oxygen is reduced to solid Li 2 O 2 , ﬁ lling the pore
D.G. Kwabi , N. Ortiz-Vitoriano , S.A. Freunberger , Y. Chen ,
N. Imanishi , P.G. Bruce , and Y. Shao-Horn
Lithium-air batteries have received extraordinary attention recently owing to their theoretical gravimetric energies being considerably higher than those of Li-ion batteries. There are, however, signifi cant challenges to practical implementation, including low energy effi ciency, cycle life, and power capability. These are due primarily to the lack of fundamental understanding of oxygen reduction and evolution reaction kinetics and parasitic reactions between oxygen redox intermediate species and nominally inactive battery components such as carbon in the oxygen electrode and electrolytes. In this article, we discuss recent advances in the mechanistic understanding of oxygen redox reactions in nonaqueous electrolytes and the search for electrolytes and electrode materials that are chemically stable in the oxygen electrode. In addition, methods to protect lithium metal against corrosion by water and dendrite formation in aqueous lithium-air batteries are discussed. Further materials innovations lie at the heart of research and development efforts that are needed to enable the development of lithium-oxygen batteries with enhanced round-trip effi ciency and cycle life.
D.G. Kwabi , Massachusetts Institute of Technology , USA ; email@example.com N. Ortiz-Vitoriano , Massachusetts Institute of Technology , USA ; firstname.lastname@example.org S.A. Freunberger , Graz University of Technology , Austria ; email@example.com Y. Chen , University of St. Andrews , UK ; firstname.lastname@example.org
spaces of the oxygen electrode in nonaqueous electrolytes and soluble LiOH in aqueous electrolytes.
The replacement of intercalation cathodes containing heavy transition metal ions that typically undergo 1 electron redox
reaction with O 2 from air that undergoes 2 electron redox
reactions offers the possibility of higher gravimetric energy.
As the O 2 is available from the air, the cost is potentially
lower than Li-ion batteries. Using nonaqueous electrolytes
and lithium as the negative electrode, Li-O 2 batteries have
an upper gravimetric energy limit of ∼ 3500
2 2 Li O
Wh/kg 3 , 7 – 10
(or ∼ 3500 Wh/kg cell considering the cell weight with lithium
and oxygen only), where oxygen is reduced to form Li 2 O 2
(2Li + O 2 ↔ Li 2 O 2 ; 2.96 V versus Li/Li + ). In contrast, Li-O 2
batteries that use aqueous electrolytes and lithium as the
negative electrode, where LiOH is formed (2Li + 1/2O 2 +
H 2 O ↔ 2LiOH; 3.2 V versus Li/Li +11 ), have lower
gravi-metric energies, with upper limits of ∼ 700–1000 Wh/kg cell
(considering the cell weight with lithium, oxygen, and seven
to twelve-fold excess water). 3 , 11 , 12 If gravimetric energy
densi-ties are calculated based on lithium metal alone, then much
higher numbers are obtained, 5 , 13 but one cannot neglect the
mass of O 2 and water.
Despite the fact that the estimated upper limits of
gravi-metric energy for Li-O 2 batteries vary depending on
dif-ferent assumptions used in the oxygen electrode 1 reported
previously, they are at least ∼ 2–3 times higher than those
of state-of-the-art Li-ion batteries. 1 – 3 It is important to
re-call that in energy storage there is no equivalent of Moore’s Law that describes a doubling of performance every 18 months in microelectronic devices (e.g., ﬂ oating point operations per second or data storage per chip footprint area). Additionally,
these large gravimetric energy gains offered by Li-O 2
chemistry can be fully realized only if lithium instead of conventional Li-ion negative elec-trode materials such as carbon is used due to the much greater gravimetric capacity of lithium (3861 mAh/g Li , Li + + e – → Li) compared
to carbon (372 mAh/g C , Li + + C 6 + e – → LiC 6 ). 14
In this article, we will consider individually the challenges and opportunities for nonaqueous
and aqueous Li-O 2 batteries, with a particular
focus on the current understanding of the reac-tion mechanisms and the materials used, which are issues that must be addressed in transforming these batteries from theory to practice.
Challenges and opportunities:
Notable progress has been made in the
develop-ment of rechargeable nonaqueous Li-O 2 batteries
in the past ﬁ ve years. Work to date has enabled prototypical labscale demonstration of signiﬁ -cant gravimetric energy density enhancements
of Li-O 2 positive electrodes ( Figure 1 a)
com-pared to state-of-the-art lithium-ion electrodes
such as LiCoO 2 , 15 LiFePO 4 , 16 and LiNi 0.5 Mn 0.5 O 2 . 17 Reported
gravimetric energy densities of cells based on oxygen elec-trodes 4 , 9 , 10 upon ﬁ rst discharge are ∼ 3 times higher than those
based on Li-ion positive electrodes ( ∼ 600 Wh/kg cell ), 17 , 18 as
shown in Figure 1b . It is important to note that the
gravi-metric energies for Li-O 2 systems only include the weight
of carbon, Li 2 O 2 , and a metallic lithium anode, which are
necessary to fairly compare the potential of the oxygen elec-trode relative to conventional Li-ion positive elecelec-trodes.
Packaged Li-O 2 cell prototypes have not been widely
devel-oped, and the true gravimetric energy advantage of practical
devices is not known. It is too early in the exploration of Li-O 2
battery technology to make accurate predictions of practical energy storage. Since the nature of the electrodes or electro-lytes that might be used in a practical system are unknown, their
tolerance to constituents in the air other than O 2 (e.g., CO 2 )
and the nature of any O 2 ﬁ ltration approaches that might have
to be taken to operate in air are also unknown. Additionally, if Li metal is used as the anode, the excess of Li that might be required in a new generation of protected Li anodes is as yet unknown. Such issues need to be investigated before hard-and-fast evidence-based estimates of practical performance can be made.
Unfortunately, rechargeable nonaqueous Li-O 2 batteries
currently suffer from low round-trip efﬁ ciency (energy deliv-ered on discharge divided by energy consumed on charge), cycle life, and power capability, 1 , 3 – 5 , 19 which limits their
practi-cal use. These performance challenges result, in part, from a lack of fundamental understanding of the mechanisms of oxygen reduction and evolution reactions in the oxygen elec-trode. Challenges also include the chemical instability of active and inactive components, including the dimensional stability
O O O O
O O O O O O
Li+ O O
O O e– e–
Figure 1. (a) Working principles of an Li-O 2 cell and (b) gravimetric Ragone plot (power
versus energy) of reported discharged Li-O 2 cells containing various carbon cathodes:
carbon nanotubes (CNTs), 8 carbon nanofi bers (CNFs), 20 and freestanding hierarchically
porous carbon (“graphene”). 10 Cells based on conventional Li-ion positive electrodes,
LiCoO 2 18 and LiNi 0.5 Mn 0.5 O 2 , 17 coupled with Li anodes for direct comparison are shown.
Note that for Li-O 2 cells, the total mass of the cathode was used (carbon + Li 2 O 2 ). Open
orange circles are for CNTs discharged to a limited capacity of 1,000 mAh/g C , while
closed orange circles are from CNT electrodes discharged to 5,000 mAh/g C . 19 The
theoretical gravimetric energy of Li 2 O 2 is calculated assuming a discharge voltage of
of metallic lithium during repeated oxidation and plating, the chemical stability of conventional current collector materials for the oxygen electrode (such as carbon), and nonaqueous electrolytes in the oxygen electrode. In the ﬁ rst part of this article, we discuss recent research ﬁ ndings that highlight the current understanding of oxygen reduction and evolution reactions in nonaqueous electrolytes and the state of the search for chemically stable nonaqueous electrolytes and porous cathode substrates.
Using vertically aligned carbon nanotubes (CNTs) as the oxygen electrode has provided valuable insights into the mechanism of oxygen reduction and evolution reactions,
speciﬁ cally Li 2 O 2 growth and oxidation mechanisms and the
relationship between Li 2 O 2 morphology/chemistry and the
voltage penalty, or overpotential, associated with Li 2 O 2 growth
and oxidation. Toroidal structures of Li 2 O 2 ( Figure 2 a), with
sizes of hundreds of nanometers, form upon discharge at
high discharge potentials (greater than 2.7 V Li ). The aspect
ratio of the toroids are scaled with the toroidal diameter, while
small Li 2 O 2 particles ( Figure 2b , <20 nm) are formed
confor-mally on CNTs at discharge voltages lower than 2.7 V Li . 10 , 20 – 22
Toroidal morphologies are characteristic of electrochemically
formed Li 2 O 2 , and they have been observed in a broad range
of non-carbonate electrolytes (ethers and dimethyl sulfoxide [DMSO]). 10 , 22 , 23 Mitchell et al. 23 have shown that these toroids
are composed of thin plates of epitaxially oriented Li 2 O 2 ,
∼ 10 nm in thickness with the
2 2 Li O
(001) direction normal to the plate surface ( Figure 2c–d ). Recent surface-sensitive x-ray absorption near edge structure (XANES) ﬁ ndings suggest that
although Li 2 O 2 is invariably formed upon battery discharge,
the electronic structure of the surfaces of the toroids have
oxygen-rich LiO 2 -like species ( Figure 2f ), while the
confor-mally coated particles retain a more stoichiometric Li 2 O 2
-related conﬁ guration. These ﬁ ndings are in agreement with recent theoretical calculations that reported the thermodynamically stable
2 2 Li O
sur-face of Li 2 O 2 , which is the dominant surface
termination of toroidal Li 2 O 2 particles, should
possess LiO 2 -like character. 24
The differences in the morphology and
surface chemistry of Li 2 O 2 particles may be
explained by the following oxygen reduction
elementary reaction steps 25 in nonaqueous
2LiO2→Li O2 2+O2
2 2 2
Li++LiO +e−→Li O
The appearance of LiO 2 as an intermediate
( Figure 2e ), followed by a disproportionation or a second electron transfer reaction to form
Li 2 O 2 , is supported in work by Peng et al. 25
using in situ surface-enhanced Raman
spec-troscopy (SERS). At high discharge potentials (low overpotentials), the growth of toroidal
Li 2 O 2 particles may involve the formation of
soluble reaction intermediate species such as O 2 – and LiO 2 and the growth of Li 2 O 2 by
chem-ical disproportion of LiO 2 . 26 , 27 These ﬁ ndings
suggest that the increasing surface area associ-ated with the increasing disc diameter during
discharge promotes Li 2 O 2 growth onto the disc
surfaces, leading to the development of thick, toroidal particles. Lowering the discharge potential (increasing the overpotential) promotes
800 900 1000 1100 1200 Raman Shift (cm–1)
OCV 3.2 V 2 min 4 min 8 min 12 min 16 min 4.4 V
1 4 1
0 200 400 600 800 1000
3.2 3.6 4.0 4.4
2.76 V (discs)
2.4 V (particles)
2.0 V (particles)
discharged at 2.5 V (particles)
Charge at 100 mA/gC
(V versus Li)
Figure 2. Transmission electron microscopy (TEM) images of carbon nanotube (CNT)
electrodes discharged at (a) 10 mA/g to 4000 mAh g C –1 showing Li 2 O 2 toroids, (b) 2.4 V to
5,000 mAh g C –1 , (c) electron diffraction patterns of toroidal Li 2 O 2 , and (d) high-resolution
TEM imaging of -oriented Li 2 O 2 plates, with lower magnifi cation in inset. Reproduced
with permission from References 19 and 23. © 2013 American Chemical Society. (e) In situ surface-enhanced Raman spectra during oxygen reduction reaction (ORR) and oxygen evolution reaction (OER) on an Au electrode in O 2 -saturated electrolyte. The peaks are
assigned as follows: (1) C–C stretch of CH 3 CN at 918 cm –1 , (2) O–O stretch of LiO 2 at
1137 cm –1 , (3) O–O stretch of Li
2 O 2 at 808 cm –1 , and (4) Cl–O stretch of ClO 4 at
931 cm –1 . Adapted with permission from Reference 25. (f) Surface-sensitive x-ray absorption
near-edge structure O–K edge data of toroids formed at 10 mA/g to 4,000 mAh g C –1
and particles formed at 2.4 V to 5,000 mAh g C –1 showing that particles closely resemble
stoichiometric Li 2 O 2 , while toroids exhibit LiO 2 -like features. (g) Constant-current charging
of Li 2 O 2 discharged at 2.0, 2.4, 2.5, and 2.76 V versus Li/Li + at 100 mA/g C , showing the
the kinetics of the second electron transfer step such that
sol-uble reaction intermediates are reduced to form Li 2 O 2
confor-mally coated on CNTs before they diffuse.
Differences in the morphology and surface chemistry
of Li 2 O 2 toroids and conformally coated particles on CNTs
appear to inﬂ uence Li 2 O 2 oxidation kinetics. 19 Upon
charg-ing at low rates, the oxidation of conformally coated Li 2 O 2
particles on CNTs exhibit a solid-solution-like voltage proﬁ le,
while oxidation of Li 2 O 2 toroids yields two-phase oxidation
with a higher voltage penalty ( Figure 2g ). Although the physi-cal origin of this observed difference is not fully understood,
it is hypothesized 19 that the oxidation kinetics of Li
2 O 2 are
dependent on surface termination. Thus, the oxidation of
Li 2 O 2 particles coated on CNTs with multiple facets can
occur at different voltages, giving rise to the sloping voltage in contrast to toroidal particles with predominantly
2 2 Li O
(001) surface terminations. This work highlights the need to under-stand how the surface chemistry and microstructure of
dis-charged Li 2 O 2 inﬂ uence oxygen evolution reaction (OER)
kinetics and opens up potential opportunities to explore
nucleation and growth mechanisms of Li 2 O 2 particles for
high-energy and/or high-power Li-O 2 batteries.
More interestingly, electron rather than lithium-ion
trans-port limits the electrochemical oxidation kinetics of Li 2 O 2 when
the oxidation current is not limited by charge transfer kinetics
under large overpotentials. This was shown in recent in situ
transmission electron microscopy (TEM) imaging experiments
with solid-state microbatteries 28 consisting of Si nanowires
(NWs) coated with Li-ion-conducting solid
electrolyte contacting Li 2 O 2 particles. In
par-ticular, as shown in Figure 3 , the oxidation of
toroidal Li 2 O 2 particles at very high
overpoten-tials is initiated preferentially at the CNT/Li 2 O 2
interface, as evidenced by the development of a light-contrast stripe beginning along the CNT axes (highlighted by the dashed red lines)
of the CNT bundle contacting the Li 2 O 2 particle.
The formation of the light-contrast stripe in
TEM can be explained by the thinning of Li 2 O 2
particles at the Li 2 O 2 /CNT interface
associ-ated with electrochemical oxidation of Li 2 O 2
(Li 2 O 2 → 2Li + + O 2 + 2e – ) and the
concur-rent release of O 2 , while lithium ions migrate
through the solid electrolyte coating the Si NW, and electrons ﬂ ow through CNTs to the Au substrate.
The preferential oxidation at the MWCNT
(multiwalled CNT)/Li 2 O 2 interface, but not
at the interface between Li 2 O 2 /solid electrolyte/
Si, suggests that electrochemical oxidation
kinetics of Li 2 O 2 is electron-transport-limited
instead of lithium-ion-transport-limited at very high overpotentials. These ﬁ ndings suggest that electrodes with large speciﬁ c surface area to
maximize the Li 2 O 2 /electrode interfacial area
and high electronic conductivity to provide facile electron transport to reaction sites are desirable for the design of
high rate rechargeable Li-O 2 batteries.
Stability of inactive components in the oxygen
Understanding the stability of inactive electrode components
in Li-O 2 batteries is an intensive area of research since their
stability is a major factor determining rechargeability and
cycle life. 29 – 35 Differential electrochemical mass spectrometry
(DEMS) experiments on isotopically labeled 13 C cathodes
have suggested that after discharge, a thin layer of Li 2 CO 3 is
present between Li 2 O 2 and carbon. 29 This hypothesis is
sup-ported by XANES studies 8 on discharged CNTs in Li-O
batteries, which show that Li 2 CO 3 is present at the interface
between Li 2 O 2 and the CNT walls on ﬁ rst discharge, and
sug-gest that carbon is not chemically stable during the oxygen reduction reaction (ORR) and is potentially reactive against Li 2 O 2 and ORR intermediates such as O 2 – and LiO 2 .
Recent in situ ambient pressure x-ray photoelectron
spectroscopy (XPS) measurements further demonstrate the
instability of carbon during ORR 30 at the interface between
graphene and a solid-state lithium ion conductor (with no nonaqueous electrolyte present). The formation of epoxy groups on the carbon surface and their conversion to
car-bonates in the presence of LiO 2 was observed and provides
direct evidence for carbon instability during battery discharge.
Interestingly, studies by Thotiyl et al. 32 using acid treatment
Figure 3. In situ transmission electron microscope (TEM) images showing oxidation of Li 2 O 2
particles. (a) Schematic illustration of the in situ TEM microbattery superimposed over a low magnifi cation TEM image of a solid electrolyte (SE)-coated Si nanowire contacting a single Li 2 O 2 particle. (b) Higher magnifi cation TEM image of the particles in (a) showing
a multiwalled carbon nanotube (MWCNT) bundle contacting two physically separated Li 2 O 2 particles labeled as Particle 1 and Particle 2, respectively. (c–g) Oxidation of
Particles 1 and 2 during application of a 10 V cell potential to the MWCNT/Li 2 O 2 positive
and Fenton’s reagent, which quantify the amounts of side-reaction products formed from decomposition of the elec-trolyte and the carbon electrode respectively, revealed that on discharge, it is the decomposition of the electrolyte not
the carbon electrode that dominates, forming Li 2 CO 3 and
carboxylate species. The degree of electrolyte decomposi-tion depends on the type of carbon used. This ﬁ nding was
further conﬁ rmed in a recent study by McCloskey et al. 31
In addition to signiﬁ cant electrolyte decomposition during ORR, they also showed that the degree of parasitic
reac-tions is sensitive to discharge rate ( Figure 4 b). 31 Further
studies are required to elucidate the reaction mechanism responsible for electrolyte decomposition with and without carbon as a function of discharge rate, carbon chemistry, and electrolyte solvent and salt.
Turning to charging, DEMS experiments with isotopic
carbon labeling show that carbon is unstable during Li 2 O 2
oxidation above 3.5 V versus Li/Li + : CO
2 is evolved, with
the carbon originating from the carbon support in the oxygen electrode ( Figure 5 a–b). 29 The analysis of 13 C labeled cathodes
at different states of charge with acid and Fenton’s reagent has revealed that the process is complex. First, while the electrolyte continues to decompose, carbon electrode
decom-position to form Li 2 CO 3 becomes signiﬁ cant and grows to
dominate at higher states of charge. The fact that carbon
decomposition commences at 3.5 V, where Li 2 O 2 starts to
oxidize signiﬁ cantly, and not at 4 V, where carbon oxidation is expected, indicates that the process of carbon
decom-position involves Li 2 O 2 or its intermediates of oxidation.
In situ DEMS shows that Li 2 CO 3 simultaneously forms by
decomposition of both the carbon cathode and the electro-lyte and decomposes on charging. As a result, the amount
of O 2 evolved on charge is not necessarily expected to be
equal to that predicted by the amount of Li 2 O 2 present at the
end of discharge. An iodometric titration method has been
developed to quantify the amount of Li 2 O 2 present in the
oxygen electrode and has conﬁ rmed this picture. When applied
at different stages of discharge and charge 31 and combined
with DEMS measurements of O 2 evolution and
consump-tion, it has been shown the Li 2 O 2 yield during charge is
con-siderably less than 100%. This ﬁ nding shows that not all
Li 2 O 2 present upon discharge evolves O 2 on charge (i.e., it
partially participates in decomposition reactions), and con-ﬁ rms that carbon is relatively more unstable during charge than discharge.
In situ ambient pressure XPS measurements have shown
highly reversible Li 2 O 2 formation on a Li x V 2 O 5 surface in
a solid-state cell, 33 thus highlighting the importance of the
design of oxygen electrodes that are stable for Li-O 2 batteries
to allow for long cycle life. In light of the observed instability of carbon, replacing it with a nanoporous gold electrode was
found to provide stable cycling of Li-O 2 batteries. 7 As Au is
heavy and expensive, TiC, TiN, Fe/N/C, N-doped carbon, and stainless steel have all been investigated as alternative
mate-rials to replace carbon. 34 Titration of each candidate cathode
after each discharge/charge with acid and Fenton’s reagent
revealed the amount of inorganic carbonates such as Li 2 CO 3
and organic carboxylate species, respectively, that were formed ( Figure 5c–d ). In comparison to carbon, TiC showed encour-aging performance and stability, which is attributed to a layer of TiOC formed on its surface. 34
Searching for stable electrolytes
Early studies of Li-O 2 battery reactions employed
carbonate-based electrolytes, where signiﬁ cant amounts of Li 2 CO 3 and
other organic side products were formed upon discharge. 35 , 36
Since then, a number of experimental 13 and computational 37
studies have shown that carbonates are highly susceptible to attack by the nucleophilic superoxide-related
species (such as O 2 – and LiO 2 ) formed during
discharge. This highlights the importance of predisposition to superoxide attack as a key design criterion in selecting stable electrolyte solvents. 13 , 25 , 35 , 38 – 40
Unlike carbonates, there are several classes
of electrolytes that support formation of Li 2 O 2
as the majority species during battery discharge ( Figure 4a ), 7 , 25 , 41 – 51 albeit with varying degrees
of side reactivity, as discussed later. This emphasizes the difﬁ culty in ﬁ nding electrolytes
stable toward the strong nucleophiles O 2 – /LiO 2
that are intermediates in Li 2 O 2 formation, as
well as toward Li 2 O 2 itself. 37 In the search for
stable electrolytes, several experimental and theoretical approaches are being pursued:
(1) Modeling of the reactions between O 2 – /
LiO 2 and the solvent (e.g., by density
func-tional theory), 37 (2) chemical screening using
KO 2 , 21 , 52 (3) electrochemical measurements
0.00 0.80 0.85 0.90 0.95
0.25 0.50 1.80
3 4 5
O2 reduction Li2O2 oxidation
Li2O2 LiHCO2 O2 O2
Li2O2/other product oxidation
Major processes Products formed
(V versus Li/Li
Figure 4. (a) Discharge-charge curve showing evolution of reaction potential ( U ) with
charge passed ( Q ) of a carbon paper-based cathode in 1 M LiTFSI (Li(CF 3 SO 2 ) 2 N) in
dimethoxyethane, along with reaction product quantifi cation during oxygen reduction reaction and oxygen evolution reaction using iodometric titration and nuclear magnetic resonance techniques. Reaction product quantifi cation shows that Li 2 O 2 is the dominant
product on discharge (along with carbonate species, R = Li or CH 3 ), while CO 2 and H 2 O
are evolved during charge as a result of electrolyte decomposition. (b) Yield of Li 2 O 2 ( YLi O22 ) as
a function of Li-O 2 battery discharge rate ( i ) for the same cathode, showing greater chemical
reactivity between Li 2 O 2 and the electrolyte at lower rates. Reprinted with permission from
(e.g., cyclic voltammetry or rotating electrodes), 41 , 53 – 56 and
(4) analysis of the reactions occurring at the cathode in a
Li-O 2 cell using a combination of spectroscopic methods
(e.g., Fourier transform infrared [FTIR], powder x-ray dif-fraction, nuclear magnetic resonance, SERS, XPS, mass spectrometry, and Li 2 O 2 titration). 7 , 42 – 44 , 57 – 59
Recent extensive investigation of nonaqueous electrolytes
for Li-O 2 cells, based on ethers, amides, ionic liquids (ILs),
and DMSO, have shown that they all predominantly support
the formation of Li 2 O 2 upon ﬁ rst discharge and its removal
on recharge. 32 , 44 – 46 Ethers are attractive for the Li–O
because they are safe, cheap, compatible with lithium metal
anodes, more stable toward reduced O 2 species compared with
organic carbonates, and have relatively high oxidation windows
(up to 4 V versus Li/Li + ), and low volatilities (for
longer-chain ethers). However, there is growing experimental and theoretical evidence that ether-based electrolytes are not suitable for Li-O 2 cells. 13 , 29 , 31 , 44 , 60 – 62 Ethers are known to form
peroxides under ambient conditions by auto
oxidation reactions. 63 This instability toward
auto oxidation has been identiﬁ ed as a possible pathway of initial attack of the solvent that gives rise to further decomposition reactions
Figure 6 b). 61
Amides are a major class of solvent that are known to be highly stable against bases and nucleophilic attack and have been extensively used for O 2 reduction studies. 64 , 65 Theoretical
calculations and KO 2 screening studies
sug-gest high-energy barriers against nucleophilic substitution at the carbons due to unfavorable
stability of the reaction products. 61
Calcu-lations also show that amides are much more stable against auto oxidation than ethers; amides require a high activation energy for proton abstraction by O 2 – . 37 Dimethylformamide (DMF)
and dimethylacetamide (DMA) have been investigated as the basis of electrolytes for
Li-O 2 batteries. 42 , 47 DMF shows greater
sta-bility than ethers, but some parasitic reac-tions occur, and signiﬁ cant capacity fading is
observed. 47 Cells with DMA electrolyte
dem-onstrate better performance, up to 80 cycles
with a reproducible voltage proﬁ le. 42
Ionic liquids and DMSO
Chemical screening by KO 2 and voltammetric
methods suggest that the stability of IL elec-trolytes is much greater than organic carbonate
solvents. 41 , 48 – 51 However, due to the difﬁ culty
of purifying ILs, the impurities that remain may be the reason for the observed parasitic reactions that compromised cycleability.
Cells based on DMSO, which have been used to study O 2
reduction in nonaqueous media in the past, 66 have shown
sus-tained cycling, with the reversible formation/decomposition of Li 2 O 2 at the cathode. 7 , 34 FTIR analysis of the discharge product
in a carbon cathode in 1M LiClO 4 in DMSO conﬁ rms dominant
formation of Li 2 O 2 , along with some Li 2 CO 3 and HCOOLi. 7 , 31 , 34 , 62
Further research on the stability of nonaqueous
electro-lytes and electrode materials in rechargeable Li-O 2 batteries
is much needed. Reactions do not proceed without side reactions; therefore, the question is not whether side reactions occur but what degree of stability is required. In this respect, two effects need to be considered: First, the extent of the side reactions, decomposition of solvent, salt, electrode, or binder to form solid, gaseous, or dissolved side products, which deplete the particular component and will lead to failure once a threshold of consumption is exceeded; and second, the nature of the side reaction products and their effects on the reversible electrochemistry. In this regard, the products of the
Figure 5. Quantifi cation of carbon-containing by-products in carbon and TiC
cathodes on discharge and charge, respectively. Data demonstrate signifi cant side reactions both on discharge and charge at carbon electrodes. These are greatly suppressed at TiC cathodes. (a) Discharge-charge curve of a carbon cathode in 0.1 M LiClO 4 /dimethyl sulfoxide electrolyte on the fi rst cycle. (b) Moles of CO 2 evolved from the
cathode stopped at certain points of discharge/charge indicated in (a) and then treated to decompose Li 2 CO 3 and lithium carboxylates. 32 (c) The same procedure applied to TiC
electrodes in the same electrolyte at the indicated numbers of discharge (1D, 5D, . . . ) and charge (1C, 5C, . . . ); shown are inorganic and organic carbonaceous products. (d) Evolution of percentage of carbonate products with cycle number at a carbon and TiC electrode, respectively. 34 Reprinted with permission from Reference 32. © 2013 American
parasitic reactions should not passivate the electrode signiﬁ -cantly (e.g., the by-products should diffuse away from the sur-face). If they cannot, they have to be able to decompose easily on charge without introducing a signiﬁ cant overpotential; otherwise, a relatively small degree of decomposition can have a dispropor-tionately large detrimental effect on the electrochemistry. This is what happens with carbon electrodes and many electrolytes,
which form solid insulating Li 2 CO 3 on the electrode surface,
leading to severe polarization and premature cell death. It may be that the combination of DMSO with a nanoporous Au cathode
produces side products other than Li 2 CO 3 , thus
avoiding large polarization.
Challenges and opportunities:
Aqueous lithium-oxygen batteriesIn the second part of this article, we will discuss recent efforts in protected lithium metal as the
negative electrode in aqueous Li-O 2 batteries.
Aqueous batteries have received signiﬁ cantly
less attention than nonaqueous Li-O 2 batteries
due to the practical challenges involved with preventing a violent reaction between lithium and water. Developing lithium metal as the neg-ative electrode that can cycle safely and stably has been a challenge for 40 years, owing to the dendrites that form on repeated lithium disso-lution and lithium deposition. Dendrites can be fatal to battery performance since they pose the risk of growing into the cathode and causing a short circuit and battery failure. There are still no rechargeable lithium anode-based batteries on the market; all rechargeable Li-ion batter-ies have thus far contained the lithium inside
another material such as aluminum (LiAl), 67 , 68
carbon (LiC 6 ), 15 , 16 , 69 and, more recently, tin 15 , 70 , 71
and silicon. 72
Zhang et al. 70 have reported lithium dendrite
formation in a typical nonaqueous electrolyte containing polyethylene glycol dimethyl ether
(PEGDME, Mw. 250) with Li(CF 3 SO 2 ) 2 N
(LiTFSI) for lithium-air rechargeable Li-O 2
batteries. The Li/PEGDME-LiTFSI/Li cell showed short circuits after 21.4 h of polarization
at 0.2 mA cm –2 and 4.0 h of polarization at
1.0 mA cm –2. A lithium metal alloy with
aluminum solved the dendrite issue, 71 but
alloy electrodes survive only a limited number of cycles owing to extreme changes in volume during operation.
To reduce lithium dendrite formation, solid electrolytes have been developed for electric
vehicle applications. 72 Theoretical calculations
suggest that a homogenous solid-state electrolyte with a modulus of 6 GPa would drastically reduce
dendrite formation. 73 As the moduli of ceramic
materials are generally higher than 6 GPa, little or no lithium dendrite formation between a ceramic lithium-ion conductor and lithium metal is expected. Visco et al. 69 and Stevens et al. 74
ﬁ rst reported experimental evidence of the feasibility of pro-tected lithium metal electrodes, with Li/Li 3 N/Li 1+ x Al x Ti 2– x (PO 4 ) 3
(LATP) and Li/Li 3– x PO 4– y N y /LATP, respectively. Li 3 N and
Li 3– x PO 4– y N y are used to prevent direct contact of lithium
metal with LATP, since LATP is electrochemically unstable at the potential of metallic lithium. 11 , 12 , 75 Aqueous Li-O
bat-teries assembled with these lithium electrodes could be cycled
Figure 6. Possible reaction schemes for ether decomposition. (a) Proposed reaction
scheme on discharge to explain decomposition of ether: electron reduction of O 2 to
superoxide (1), binding with Li + (2), and disproportionation to Li
2 O 2 (3) as the ideal
sequence. Alternatively, superoxide may abstract a proton from the solvent (4) to give hydroperoxide (5), which may further react in a series of oxidative decomposition steps (6) or yield esters or polymeric compounds (7). Superoxide and CO 2 from step (6) react to
form Li 2 CO 3 (8 and 9). (b) Alternative possible pathway with initial attack by autoxidation
to give hydroperoxyl and alkyl radicals (I) and chain propagation by O 2 addition and further
proton abstraction (II and III). Note: The dot ( • ) denotes a free radical. (a) Reprinted with
at 1 mA cm –2 and room temperature without degradation
of the cell performance for a short period of 10 min. 69 , 73
Subsequently, other protected lithium anodes based on
gar-net-type solid electrolytes 76 and polymer-ceramic composite
membranes 77 have been reported.
While ceramic conductors are stiff enough to prevent lith-ium dendrite growth, they do not easily make low-resistance contacts with other solid components and thus have high charge transfer resistance. Recent research efforts have been focused on using polymer-ceramic composite electrolytes to form a conformal interface and reduce interfacial resistance. Rosso et al. investigated the mechanism of lithium dendrite growth in Li/PEO-based-electrolyte/Li (PEO = polyethylene
oxide), 78 , 79 where the onset of dendrite formation and the time
to reach short-circuit times can be studied by direct in situ
observation and simultaneous cell voltage monitoring. Table I
summarizes the dendrite onset and short-circuit time for dif-ferent compositions of PEO-based electrolytes. No dendrite
formation was observed in a Li/PEO 20 LiTFSI/Li cell at a low
current density of 0.03 mA cm –2 for 100 h at 80°C, while at a
high current density of 0.7 mA cm –2 , dendrites were observed
after less than 1 h of deposition. 79 Such lithium dendrite
formation onset times at high current density are too short to be used in practical applications. The use of ceramic or IL additives in polymer electrolytes comprises another strategy to
suppress dendrite formation. The addition of nano-SiO 2 and/
or IL of N -methyl- N -propylpiperidinium TFSI (PP13TFSI) 80 , 81
to polymer electrolytes has been shown to increase the onset
time of dendrite formation from 10 h for Li/PEO 18 TFSI/Li to
21 h at 1.0 mA cm –2 at 60°C. Figure 7 a shows the cycling
performance of the lithium deposition and dissolution process
in a Li/PEO 18 LiTFSI-SiO 2 -PP13TFSI/Li cell at 60°C, where
the cell voltage showed no signiﬁ cant change during cycling, and no dendrite formation was detected at a current density of 0.3 mA cm –2 for 30 h. 81
Based on these positive results, this composite polymer
elec-trolyte of PEO 18 LiTFSI-SiO 2 -PP13TFSI was also assessed as the
protected lithium-metal anode for rechargeable lithium-air
bat-teries. Figure 7b shows reversible cycling of a Li/PEO 18
LiTFSI-PP13TFSI/LATP/aqueous 1 M LiCl-0.004 M LiOH/Pt, air cell
at 0.3 mA cm –2 and 60°C, 82 with LATP as the solid electrolyte.
The inclusion of PP13TFSI IL is effective in reducing interfa-cial resistance between lithium and the electrolyte and
facili-tating highly reversible Li-O 2 cycling.
While the early onset of lithium dendrite formation and low output power remain yet to be completely solved, recent research has shown that these challenges are closely related to the physical properties of the solid electrolyte used. Further materials devel-opment for the protection layer of lithium is therefore essential
to achieve high power density at several mA cm –2 and extended
deep cycling of the lithium electrode for Li-O 2 batteries.
The need for storage technologies with much greater gravimetric
energy than Li-ion batteries makes Li-O 2 batteries an attractive
energy storage option for applications that require high-energy density such as electric vehicles. Although notable progress has been made in the development of rechargeable, lab-scale
non-aqueous Li-O 2 cells, further investigation of the oxygen
reduc-tion reacreduc-tion (ORR) and oxygen evolureduc-tion reacreduc-tion (OER) in nonaqueous electrolytes, and parasitic reaction mechanisms in-volving inactive components in the oxygen electrode is required
in order to aid the rational design and development of kinetically facile and chemically stable electrode and electro-lyte conﬁ gurations.
As detailed in this review, research-ers have just begun to connect the phys-ical properties (morphology and surface
versus bulk chemistry) of Li 2 O 2 with
the corresponding kinetics of Li 2 O 2
for-mation and oxidation. Important topics warranting further investigation in this area include the detailed reaction and
growth mechanisms of Li 2 O 2 at high
and low overpotentials; the electronic nature (surface and bulk) of electro-chemically formed Li 2 O 2 ; intrinsic Li 2 O 2
oxidation pathways; and the inﬂ uence of non-carbonate solvents on the nucleation
and growth of Li 2 O 2 and its oxidation.
As carbon is not stable in the oxy-gen electrode, improved morphological, chemical, and kinetic understanding of
Li-O 2 reactions in non-carbon electrodes
will become increasingly relevant for
Table I. Dependence of lithium dendrite formation onset time ( t o ) and short-circuit time ( t s )
on electrolyte formulation, temperature, and current density.
(mAcm −2 )
Onset time (hour)
Short circuit time (hour)
(Li/O = 1/20) room
0.2 21 70
(Li/O = 1/20)- 20 room
0.2 110 70
wt% SiO 2 1.0 20
PVdF-HFP-SiO 2 -EC-PC- room
0.6 14 83
PEO-LiTFSI (Li/O = 1/20) 80 0.05 38 110 78
PEO 18 LiTFSI-1.44PP13TFSI 60 0.1 125 235 80
1.0 10 15
PEO 18 LiTFSI-1.44PP13TFSI- 60 0.1 460 672 84
10 wt% SiO 2 1.0 21 37
Note: PVdF, polyvinylidene ﬂ uoride; HFP, hexaﬂ uorophosphate; EC, ethylene carbonate; PC, propylene carbonate; PEO, polyethylene oxide; LiTFSI, Li(CF 3 SO 2 ) 2 N; PEGDME, polyethylene glycol dimethyl ether;
the development of rechargeable Li-O 2 batteries. The search
for electrolytes that are chemically stable against the oxygen electrode is another major focus of research. The discovery that reduced oxygen species produced during ORR are also highly reactive against a broad range of electrolyte solvents has spurred detailed spectroscopic, spectrometric, and titration studies examining the interplay between electrolyte formulation and discharge reaction product. Combining these experimental approaches with theoretical calculations evaluating electrolyte
susceptibility to attack by Li 2 O 2 and/or ORR intermediates
will be crucial to ﬁ nding an electrolyte that is moderately sta-ble during ORR, but also possesses a favorasta-ble synergy with the chosen electrode material such that parasitic reactions during OER are minimized.
Signiﬁ cant progress has been made toward ﬁ nding materials that suppress lithium dendrite formation and also adequately protect the lithium metal anode from contact with reactive gases and water in both nonaqueous and aqueous
Li-O 2 battery environments. Representing a compromise
between the favorable transport properties of liquid and the high mechanical stability of solid electrolytes, the use of polymers has emerged as a particularly promising strategy to protect lithium metal anodes. Further research into the possibility of incorporating nanostructured additives to improve power capabilities while maintaining chemical
stability against lithium metal in full Li-O 2 cells is a promising
direction for future efforts in this ﬁ eld. The need for funda-mentally understanding the relationship between electrode reaction mechanisms and parasitic processes occurring in
rechargeable Li-O 2 batteries presents an opportunity to combine
cutting edge experimental and computational techniques with materials innovation in the areas outlined previously to enable
the development of practical rechargeable Li-O 2 batteries, which
combine high rate capability with high round-trip efﬁ ciency and long cycle life.
Y.S-H., N.O.-V. and D.G.K. gratefully acknowl-edge the Robert Bosch Company for a Bosch Energy Research Network Grant, the CERC-CVC US China Clean Energy Research Center-Clean Vehicles Consortium of the Department of
Energy (under award number DE — PI0000012),
and the MRSEC program of the National Science Foundation for their generous support
(under award number DMR — 0819762). N.O.-V.
acknowledges a Marie Curie International Out-going Fellowship within the seventh European Community Framework Programme (2012). P.G.B. acknowledges the EPSRC for ﬁ nancial support, including the SUPERGEN program. S.A.F. acknowledges ﬁ nancial support by the Austrian Federal Ministry of Economy, Family and Youth and the Austrian National Foundation for Research, Technology and Development.
1. Y.-C. Lu , B.M. Gallant , D.G. Kwabi , J.R. Harding , R.R. Mitchell , M.S. Whittingham , Y. Shao-Horn , Energy Environ. Sci. 6 , 750 ( 2013 ).
2. J.-S. Lee , S. Tai Kim , R. Cao , N.-S. Choi , M. Liu , K.T. Lee , J. Cho , Adv. Energy Mater. 1 , 34 ( 2011 ).
3. P.G. Bruce , S.A. Freunberger , L.J. Hardwick , J.-M. Tarascon , Nat. Mater. 11 , 19 ( 2012 ).
4. J. Christensen , P. Albertus , R.S. Sanchez-Carrera , T. Lohmann , B. Kozinsky , R. Liedtke , J. Ahmed , A. Kojic , J. Electrochem. Soc. 159 , R1 ( 2012 ). 5. P.G. Bruce , L.J. Hardwick , K.M. Abraham , MRS Bull. 36 , 506 ( 2011 ). 6. Y. Shao , S. Park , J. Xiao , J.-G. Zhang , Y. Wang , J. Liu , ACS Catal. 2 , 844 ( 2012 ).
7. Z. Peng , S.A. Freunberger , Y. Chen , P.G. Bruce , Science 337 , 563 ( 2012 ). 8. B.M. Gallant , R.R. Mitchell , D.G. Kwabi , J. Zhou , L. Zuin , C.V. Thompson , Y. Shao-Horn , J. Phys. Chem. C 116 , 20800 ( 2012 ).
9. S.H. Oh , L.F. Nazar , Adv. Energy Mater. 2 , 903 ( 2012 ).
10. Z.-L. Wang , D. Xu , J.-J. Xu , L.-L. Zhang , X.-B. Zhang , Adv. Funct. Mater. 22 , 3699 ( 2012 ).
11. S. Hasegawa , N. Imanishi , T. Zhang , J. Xie , A. Hirano , Y. Takeda , O. Yamamoto ,
J. Power Sources 189 , 371 ( 2009 ).
12. N. Imanishi , S. Hasegawa , T. Zhang , A. Hirano , Y. Takeda , O. Yamamoto ,
J. Power Sources 185 , 1392 ( 2008 ).
13. B.D. McCloskey , D.S. Bethune , R.M. Shelby , G. Girishkumar , A.C. Luntz ,
J. Phys. Chem. Lett. 2 , 1161 ( 2011 ).
14. H. Ikeda , R. Hoch , R. Hausslein , US Patent 05879836 ( 1999 ). 15. H. Xia , L. Lu , G. Ceder , J. Power Sources 159 , 1422 ( 2006 ). 16. Y. Zhu , C. Wang , J. Phys. Chem. C 114 , 2830 ( 2010 ).
17. K. Kang , Y.S. Meng , J. Bréger , C.P. Grey , G. Ceder , Science 311 , 977 ( 2006 ). 18. H. Chen , M. Armand , G. Demailly , F. Dolhem , P. Poizot , J.-M. Tarascon ,
ChemSusChem 1 , 348 ( 2008 ).
19. B.M. Gallant , D.G. Kwabi , R.R. Mitchell , J. Zhou , C.V. Thompson , Y. Shao-Horn ,
Energy Environ. Sci. 6 , 2518 ( 2013 ).
20. R.R. Mitchell , B.M. Gallant , C.V. Thompson , Y. Shao-Horn , Energy Environ. Sci. 4 , 2952 ( 2011 ).
21. R. Black , S.H. Oh , J. Lee , T. Yim , B. Adams , L.F. Nazar , J. Am. Chem. Soc.
134 , 2902 ( 2012 ).
22. D. Xu , Z. Wang , J. Xu , L. Zhang , X. Zhang , Chem. Commun. 48 , 6948 ( 2012 ).
23. R.R. Mitchell , B.M. Gallant , Y. Shao-Horn , C.V. Thompson , J. Phys. Chem. Lett. 4 , 1060 ( 2013 ).
24. J.S. Hummelshøj , A.C. Luntz , J.K. Nørskov , J. Chem. Phys. 138 , 034703 ( 2013 ).
25. Z. Peng , S.A. Freunberger , L.J. Hardwick , Y. Chen , V. Giordani , F. Bardé , P. Novák , D. Graham , J.-M. Tarascon , P.G. Bruce , Angew. Chem. Int. Ed. Engl.
50 , 6351 ( 2011 ).
670 680 690 700 710 720 0.0
0 1 2
200 400 600 800 1000 1200 1400 1600 1800
Potential (V) Time (h)
with SiO2 +PP13TFSI
Time (Hour) a
WSLE Potential (V)
Figure 7. (a) Cycling performance for the Li/PEO 18 LiTFSI-SiO 2 -PP13TFSI/Li cell at 0.3
mA cm –2 and 60°C. The inset shows a comparison of the 11th cycle for Li/PEO 18
LiTFSI-SiO 2 -PP13TFSI/Li and Li/PEO 18 LiTFSI-PP13TFSI/Li. Cycling performance of the Li/
PEO 18 LiTFSI-1.44PP13TFSI/LATP/aqueous 1 M LiCl-0.004 M LiOH/Pt-air cell at 0.3 mA cm –2
and 60°C between (b) 0 h and 400 h. The water-stable lithium electrode (WSLE) voltage was measured by a Pt-air reference electrode. Discharge and charge period are both two hours. Cycle was repeated without interval. Microscopic observations of the cell indicated no dendrite formation after cycling. Note: PEO, polyethylene oxide; LiTFSI, Li(CF 3 SO 2 ) 2 N; PP13, N -methyl- N -propylpiperidinium; LATP, Li 1+ x Al x Ti 2– x (PO 4 ) 3 . (a) Reprinted
26. B.D. Adams , C. Radtke , R. Black , M.L. Trudeau , K. Zaghib , L.F. Nazar , Energy Environ. Sci. 6 , 1772 ( 2013 ).
27. D. Zhai , H.-H. Wang , J. Yang , K.C. Lau , K. Li , K. Amine , L.A. Curtiss , J. Am.
Chem. Soc. 135 , 15364 ( 2013 ).
28. L. Zhong , R.R. Mitchell , Y. Liu , B.M. Gallant , C.V. Thompson , J.Y. Huang , S.X. Mao , Y. Shao-Horn , Nano Lett. 13 , 2209 ( 2013 ).
29. B.D. McCloskey , A. Speidel , R. Schefﬂ er , D.C. Miller , V. Viswanathan , J.S. Hummelshøj , J.K. Nørskov , A.C. Luntz , J. Phys. Chem. Lett. 3 , 997 ( 2012 ).
30. D.M. Itkis , D.A. Semenenko , E.Y. Kataev , A.I. Belova , V.S. Neudachina , A.P. Sirotina , M. Hävecker , D. Teschner , A. Knop-Gericke , P. Dudin , A. Barinov , E.A. Goodilin , Y. Shao-Horn , L.V. Yashina , Nano Lett. 13 , 4697 ( 2013 ). 31. B.D. McCloskey , A. Valery , A.C. Luntz , S.R. Gowda , G.M. Wallraff , J.M. Garcia , T. Mori , L.E. Krupp , J. Phys. Chem. Lett. 4 , 2989 ( 2013 ).
32. M.M. Ottakam Thotiyl , S.A. Freunberger , Z. Peng , P.G. Bruce , J. Am. Chem. Soc. 135 , 494 ( 2012 ).
33. Y.-C. Lu , E.J. Crumlin , G.M. Veith , J.R. Harding , E. Mutoro , L. Baggetto , N.J. Dudney , Z. Liu , Y. Shao-Horn , Sci. Rep. 2 , 715 ( 2012 ).
34. M.M. Ottakam Thotiyl , S.A. Freunberger , Z. Peng , Y. Chen , Z. Liu , P.G. Bruce ,
Nat. Mater. 12 , 1050 ( 2013 ).
35. F. Mizuno , S. Nakanishi , Y. Kotani , S. Yokoishi , H. Iba , Electrochemistry 78 , 403 ( 2010 ).
36. W. Xu , V.V. Viswanathan , D. Wang , S.A. Towne , J. Xiao , Z. Nie , D. Hu , J.-G. Zhang , J. Power Sources 196 , 3894 ( 2011 ).
37. V.S. Bryantsev , J. Uddin , V. Giordani , W. Walker , D. Addison , G.V. Chase ,
J. Electrochem. Soc. 160 , A160 ( 2012 ).
38. D.T. Sawyer , J.L. Roberts , Jr ., J. Electroanal. Chem. 12 , 90 ( 1966 ). 39. C.O. Laoire , S. Mukerjee , K.M. Abraham , E.J. Plichta , M.A. Hendrickson ,
J. Phys. Chem. C 113 , 20127 ( 2009 ).
40. R. Younesi , M. Hahlin , F. Björefors , P. Johansson , K. Edström , Chem. Mater.
25 , 77 ( 2012 ).
41. J. Herranz , A. Garsuch , H.A. Gasteiger , J. Phys. Chem. C 116 , 19084 ( 2012 ).
42. W. Walker , V. Giordani , J. Uddin , V.S. Bryantsev , G.V. Chase , D. Addison ,
J. Am. Chem. Soc. 135 , 2076 ( 2013 ).
43. F. Mizuno , K. Takechi , S. Higashi , T. Shiga , T. Shiotsuki , N. Takazawa , Y. Sakurabayashi , S. Okazaki , I. Nitta , T. Kodama , H. Nakamoto , H. Nishikoori , S. Nakanishi , Y. Kotani , H. Iba , J. Power Sources 228 , 47 ( 2013 ).
44. S.A. Freunberger , Y. Chen , N.E. Drewett , L.J. Hardwick , F. Bardé , P.G. Bruce ,
Angew. Chem. Int. Ed. Engl. 50 , 8609 ( 2011 ).
45. C. Laoire , S. Mukerjee , E.J. Plichta , M.A. Hendrickson , K.M. Abraham ,
J. Electrochem. Soc. 158 , A302 ( 2011 ).
46. M. Leskes , N.E. Drewett , L.J. Hardwick , P.G. Bruce , G.R. Goward , C.P. Grey ,
Angew. Chem. Int. Ed. Engl. 51 , 8560 ( 2012 ).
47. Y. Chen , S.A. Freunberger , Z. Peng , F. Bardé , P.G. Bruce , J. Am. Chem. Soc.
134 , 7952 ( 2012 ).
48. F. Mizuno , S. Nakanishi , A. Shirasawa , K. Takechi , T. Shiga , H. Nishikoori , H. Iba , Electrochemistry 79 , 876 ( 2011 ).
49. K. Takechi , S. Higashi , F. Mizuno , H. Nishikoori , H. Iba , T. Shiga , ECS Elec-trochem. Lett. 1 , A27 ( 2012 ).
50. S. Monaco , A.M. Arangio , F. Soavi , M. Mastragostino , E. Paillard , S. Passerini ,
Electrochim. Acta 83 , 94 ( 2012 ).
51. C.J. Allen , J. Hwang , R.A. Kautz , S. Mukerjee , E.J. Plichta , M.A. Hendrickson , K.M. Abraham , J. Phys. Chem. C 116 , 20755 ( 2012 ).
52. K.U. Schwenke , S. Meini , X. Wu , H.A. Gasteiger , M. Piana , Phys. Chem.
Chem. Phys. 15 , 11830 ( 2013 ).
53. D. Aurbach , M. Daroux , P. Faguy , E. Yeager , J. Electroanal. Chem. Interfacial
Electrochem. 297 , 225 ( 1991 ).
54. V.S. Bryantsev , V. Giordani , W. Walker , M. Blanco , S. Zecevic , K. Sasaki , J. Uddin , D. Addison , G.V. Chase , J. Phys. Chem. A 115 , 12399 ( 2011 ). 55. C.O. Laoire , S. Mukerjee , K.M. Abraham , E.J. Plichta , M.A. Hendrickson ,
J. Phys. Chem. C 114 , 9178 ( 2010 ).
56. C.J. Allen , S. Mukerjee , E.J. Plichta , M.A. Hendrickson , K.M. Abraham ,
J. Phys. Chem. Lett. 2 , 2420 ( 2011 ).
57. H.-G. Jung , J. Hassoun , J.-B. Park , Y.-K. Sun , B. Scrosati , Nat. Chem. 4 , 579 ( 2012 ).
58. Y.-C. Lu , H.A. Gasteiger , Y. Shao-Horn , J. Am. Chem. Soc. 133 ( 47 ), 19048 ( 2011 ).
59. S.H. Oh , R. Black , E. Pomerantseva , J.-H. Lee , L.F. Nazar , Nat. Chem. 4 , 1004 ( 2012 ).
60. R. Younesi , M. Hahlin , M. Treskow , J. Scheers , P. Johansson , K. Edstrom ,
J. Phys. Chem. C 116 , 18597 ( 2012 ).
61. V.S. Bryantsev , F. Faglioni , J. Phys. Chem. A 116 , 7128 ( 2012 ).
62. K.R. Ryan , L. Trahey , B.J. Ingram , A.K. Burrell , J. Phys. Chem. C 116 , 19724 ( 2012 ).
63. A.M. Clover , J. Am. Chem. Soc. 44 , 1107 ( 1922 ).
64. D.T. Sawyer , J.S. Valentine , Acc. Chem. Res. 14 , 393 ( 1981 ). 65. M.E. Peover , B.S. White , Electrochim. Acta 11 , 1061 ( 1966 ). 66. M.V Merritt , D.T. Sawyer , J. Org. Chem. 35 , 2157 ( 1970 ).
67. Y.-I. Jang , B.J. Neudecker , N.J. Dudney , Electrochem. Solid-State Lett. 4 , A74 ( 2001 ).
68. M.D. Levi , D. Aurbach , J. Phys. Chem. B 101 , 4630 ( 1997 ).
69. S. Visco , B. Katz , M.Y. Chu , L. De Jonghe , Eds., Symposium on Scalable Energy
Storage: Beyond Lithium-Ion ( IBM, Almaden Institute , San Jose, CA 2009 ).
70. X.-W. Zhang , Y. Li , S.A. Khan , P.S. Fedkiw , J. Electrochem. Soc. 151 , A1257 ( 2004 ).
71. B.M.L. Rao , R.W. Francis , H.A. Christopher , J. Electrochem. Soc. 124 , 1490 ( 1977 ).
72. S. Megahed , B. Scrosati , Electrochem. Soc. Interface 4 , 34 ( 1995 ). 73. C. Monroe , J. Newman , J. Electrochem. Soc. 152 , A396 ( 2005 ).
74. P. Stevens , G. Toussaint , G. Caillon , P. Viaud , P. Vinatier , C. Cantau , O. Fichet , C. Sarrazin , M. Mallouki , ECS Trans. 28 , 1 ( 2010 ).
75. D. Capsoni , M. Bini , S. Ferrari , E. Quartarone , P. Mustarelli , J. Power Sources 220 , 253 ( 2012 ).
76. R. Murugan , V. Thangadurai , W. Weppner , Angew. Chem. Int. Ed. Engl. 46 , 7778 ( 2007 ).
77. B. Kumar , J. Kumar , R. Leese , J.P. Fellner , S.J. Rodrigues , K.M. Abraham ,
J. Electrochem. Soc. 157 , A50 ( 2010 ).
78. M. Rosso , T. Gobron , C. Brissot , J.-N. Chazalviel , S. Lascaud , J. Power Sources 97 – 98 , 804 ( 2001 ).
79. C. Brissot , M. Rosso , J.-N. Chazalviel , S. Lascaud , J. Power Sources 81 – 82 , 925 ( 1999 ).
80. S. Liu , N. Imanishi , T. Zhang , A. Hirano , Y. Takeda , O. Yamamoto , J. Yang ,
J. Electrochem. Soc. 157 , A1092 ( 2010 ).
81. S. Liu , H. Wang , N. Imanishi , T. Zhang , A. Hirano , Y. Takeda , O. Yamamoto , J. Yang , J. Power Sources 196 , 7681 ( 2011 ).
82. T. Zhang , N. Imanishi , A. Hirano , Y. Takeda , O. Yamamoto , Electrochem. Solid-State Lett. 14 , A45 ( 2011 ).
83 L. Sannier , R. Bouchet , M. Rosso , J.-M. Tarascon , J. Power Sources 158 , 564 ( 2006 ).
84. W. Xu , K. Xu , V.V. Viswanathan , S.A. Towne , J.S. Hardy , J. Xiao , Z. Nie , D. Hu , D. Wang , J.-G. Zhang , J. Power Sources 196 , 9631 ( 2011 ).
A publication of the
CALL FOR PAPERSFebruary 2015 Issue
June 15, 2014